6; 3 )// ALLOY COMPATIBILITY WITH LiF-BeF, SALTS CONTAINING ThF, A N D UF, J. W . Koger
This report was prepared as an account of work sponsored by the United States Government. Neither the United States nor the United States Atomic Energy Commission, nor any of their employees, nor any of their contractors, subcontractors, or their employees, makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness or usefulness of any information, apparatus, product or process disclosed, or represents that i t s use would not infringe privately owned rights.
Contract No. W-7405-eng-26
METALS AND CERAMICS DIVISION
ALLOY COMPATIBILITY WITH LiF-BeF, SALTS CONTAINING ThF4 AND UF4 J. W. Koger
NOTICE This report was prepared as an account of work sponsored by the United States Government. Neither the United States nor the United States Atomic Enerw Commission, nor any of their employees, nor any Of their contractors, subcontractors, or their employees, makes any warranty, express o r implied. or assumes any legal liability or responsibility for the accuracy, completeness o r usefulness of any information, apparatus, product o r process disclosed, o r represents that Its use would not infringe privately owned rights.
OAK RIDGE NATIONAL LABORATORY Oak Ridge, Tennessee 37830 operated by UNION CARBIDE CORPORATION for the US. ATOMIC ENERGY COMMISSION
tflSTRlBUTlON OE THIS DOCUMENT IS U
Materials Selection and Fabrication
........................................................................... Hastelloy N .................................................................... Loop15 .................................................................... LooplSA ................................................................... Loops18and19 ............................................................. Loop21 .................................................................... Loop 16A ................................................................... Type304LStainlessSteel ......................................................... Loop1258 .................................................................. MaragingSteel .................................................................. Type316StainlessSteel ........................................................... Loop22 .................................................................... OtherAlloys .................................................................... Loopl8A ...................................................................
11 11 15 17 23 27
28 28 33 36 36 40
ALLOY COMPATIBILITY WITH LiF-BeFz SALTS CONTAINING ThF4 AND UF4 J. W. Koger
Various compatibility tests between LiF-BeF2-based salts and Hastelloy N and certainsteels were conducted in thermal convection loops. Temperature gradient mass transfer, as noted by weight losses in the hot leg and weight gains in the cold leg, was evidenced in all tests. The weight changes of corrosion specimens increased with increasing temperature and time. From an o p e ~ i ~ t i standpoint, o~l some difficulty was encountered in melting LiF-BeF2-ThF4 salt without mechanically failing the loop. The difficulty stemmed from the high melting point of the salt and the high melting point of certain phases in the salt. AU the salts tested were quite compatible with Hastelloy N. Bismuth in contact with a fuel salt had no effect on mass transfer in a Hastelloy N loop. We established that electrochemical methods to determine the oxidation potential of molten fluoride salts could be used to predict the corrosion behavior of a thermal convection loop. The values obtained by the electrochemical methods correlated well with specimen weight change data. We showed that tellurium (as plated on Hastelloy N specimens) does mass transfer in a molten fluoride salt system and that an equilibrium between tellurium in the salt and tellurium on the alloy can be established. A type 304L stainless exposed to a fuel salt for 9.5 years in a type 304L stainless steel loop showed a maximum uniform corrosion rate of 0.86 mil/year. Voids extended 10 mils into the matrix. Chromium depletion was found. The corrosion resistance of maraging steel (12%Ni-5% Cr-3% Mo-bal Fe) at 662OC was better than type 304L stainless but worse than Hastelloy N under equivalent conditions. The uniform corrosion rate w a s 0.55 mil/year. Subsurface voids were seen in the microstructure of the specimens after 5700 hr, and microprobe analysis disclosed a definite depletion of chromium and iron. Type 316 stainless steel exposed to a fuel salt in a type 316 stainless steel loop showed a maximum uniform corrosion rate of 1 mil/year for 4298 hr. Mass transfer of chromium and iron did occur in the system. For selected nickel- and iron-base alloys a direct correlation was found between corrosion re,sistance in a molten fluoride salt and the chromium and kon content of an alloy. The more chromium and iron in the alloy, the less the corrosion resistance.
INTRODUCTION A large portion of the support work of the Molten-Salt Breeder Reactor (MSBR) Program involved studies of the compatibility and mass transfer of various alloys with LiF-BeF2-based molten salts. Table 1 gives the alloys involved, the salt compositions, and the details of the tests. Many of these tests were conducted in thermal convection loops like that shown schematically in Fig. 1. The loops are essentially Table 1. Thermal convection loop experiment6 involvingLiF-BeF2-based molten salts Loop No.
1258 15 1SA 1gb 16A 18 18A 19 19A 21 22
Salt composition (mole %) LiF-BeF2-ZrF4-UF4-ThF4 (70-23-5-1-1) LiF-BeFz-ThFe (73-2-25) LiF-BeFz-ThF4 (7 3-2-25) LiF-BeF2-UF4 (65.5-34-0.5) LiF-BeFz-UF4 (65 5-34-05) LiF-BeF2-ThF4-UF4 (68-20-11.7-0.3) LiF-BeFz-ThF4-UF4 (68-20-11.7-0.3) LiF-BeFz-ThFh-UF, (68-20-11.7-0.3) LiF-BeFz-ThF4-UFd (68-20-11.7-0.3) LiF-BeFz-ZrF4-UF4 (65.4-29.1-5-0) LiF-BeFz-ThF4-UF4 (68-20-11.7-0.3)
688 677 677 704 704 704 704 104 704 610 650
100 55 55 170 170 170 170 170 170 110 110
83,516 2,003 39,476 37,942 5.878 15,930 2,278 4,745 24,515 13,798 4,491
aLoop 1258 constructed of type 304L stainless steel; loop 22 constructed of type 316 stainless steel; all other loops constructed of Hastelloy N. bThis loop is discussed in another report, J. W. Koger, Effect of FeF2 Addition on Mass Tkansfer in a Hastelloy N-LiF-BeF2-UF4 Thermal Convection Loop System, ORNL-TM4188 (December 1972).
Fig. 1. MSRP natural circulation loop and salt sampler.
3 test bed systems wherein metal specimens suspended in the salt and salt samples can be removed and/or replaced at operating temperature without disturbing flow or introducing air contamination. The salt flow in the thermal convection loops is generated by the difference in density of the salt in the hot and cold legs of the loop and ranges from 1.5 to 7 ft/min depending on salt density and viscosity. A thorough chemistry background and physical properties of the molten salts are covered elsewhere by Grimes. MOLTEN SALT CHEMISTRY Uranium tetrafluoride and uranium trifluoride are the only fluorides of uranium which appear useful as constituents of molten fluoride fuels. Uranium tetrafluoride (UF,) is relatively stable, nonvolatile, and nonhygroscopic. It melts at 1035°C (1895”F), but its freezing point is markedly depressed by useful diluent fluorides. Uranium trifluoride disproportionates at temperatures above -1000°C by the reaction
4UF3+ 3UF4 + Uo.
It is chemically unstable293 at lower temperatures in most molten fluoride solutions and is tolerable in reactor fuels only with a large excess of UF4 so that the activity of Uo is so low as to avoid appreciable reaction with moderator graphite or container metal. Thorium tetrafluoride (ThF4) is the only known fluoride of thorium. It melts at 1111°C (2032”F), but fortunately its freezing point is markedly depressed by fluoride diluents which are also useful with UF4 . Consideration of nuclear properties alone leads one to prefer as diluents the fluorides of Be, Bi, ‘Li, Mg, Pb, and Zr in that order. Simple consideration of the stability of these fluorides495 toward reduction by structural metals, however, eliminates the bismuth fluorides from consideration. This leaves BeF, and ‘LiF as the preferred diluent fluorides. Phase behavior of systems based upon LiF and BeF2 as the major constidents has, accordingly, been examined in detail.6 Fortunately the phase diagrams of LiF-BeF2-UF4 and LiF-BeF2-ThF4 are such as to make these materials useful as fuels. The binary system LiF-BeF, has melting points below 500°C over the concentration range from 33 to 80 mole % BeF2.6*7 The phase diagram presented in Fig. 2 is characterized by a single eutectic (52 mole % BeF,, melting at 360°C) between BeF, and 2LiF*BeF2. The compound 2LiF*BeF2 melts incongruently to LiF and liquid at 458°C. LiF*BeF2 melts below 280°C. The phase behavior of the BeF2-UF46s7 and BeF2-ThF4E systems is very similar. Both systems show simple single eutectics containing very small concentrations of the heavy metal fluoride. ThF4 and UF4 are isostructural; they form a continuous series of solid solutions. The binary diagrams LiF-UF4 and LiF-ThF4 are generally simiiar and much more complex than the binary diagrams just discussed. The LiF-UF4 system has three compounds (none of which melt 1. W. R. Grimes, “Molten-Salt Reactor Chemistry,”Nucl. Appl. Technol. 8,137 (1970). 2. W. R. Grimes, “Materials Problems in Molten Salt Reactors7 in Materials and Fuels for High TemperatureNuclear Energy Applications, M. T. Simnad and L. R. Zumwalt, eds., the M.I.T. Press, Mass. (1964). 3. W. R. Grimes,MSR Program Semiannu. Progr. Rep. July 31.1964,ORNL-3708, p- 214. 4. Alvin Glassner, The ThermochemicalProperties of the Oxides, Fluorides, and Chlorides to 25OO0K. ANL-5750. 5. L. Brewer, L. A. Bromley, P. W. Cilleg, and N. L. Lofgren, MDDC-1553 (1945) and L. Brewer in The Chemistry and Metallurgy of Miscelkzneous Materhls, Thermodynamics, L. L. Quill, led., McGraw-Hill, New York,pp. 76-192 (1950). 6. R.E.Thoma,Phase Diagrams ofNucIear Reactor Materrhls, ORNL-2548 (Nov.6,1959). 7. L. V. Jones, D.E. Etter, C. R. Hudgens, A. A. Huffman,T. B. Rhinehammer, N. E. Rogers, P.A.Tucker, and L. J. Wittenberg, “Phase Equilibria in the Ternary Fused-Salt System LiF-BeF2-UF4,”J. Amer. Cerum. SOC.45,79 (1962). 8. R. E. Thoma, H. Insley, H. A. Friedman, and C. F. Weaver, “Phase Equilibria in the Systems BePz-ThF4 and LiF-BeFz-ThF4,”J. Phys. Chem 64,865 (1960). 9. C. J. Barton, H. A. Friedman, W. R. Grimes, H. Insley, and R. E. Thoma, “Phase Equilibria in the Alkali Fluoride-Uranium Tetrafluoride Fused Salt System: 1. The Systems LiF-UF4 and NaF-UF4,”J. Amer. Ceram. Soc. 41,63 (1958). 10. R. E. Thoma, H. Insley, B. S. Landau, H.A. Friedman, and W. R. Grimes, “Phase Equilibria in the Fused Salt Systems LiF-ThF4 and NaF-ThF4,”J. Phys. Chem 63,1266 (1959).
4 ORNL-DWG 71-597ORZ
I 700 I
500 BeF, (@-OUARTZ TYPE1
XBeF, (mole froction)
Fig. 2. The system LiF-BeF2.
congruently) and a single eutectic at 27 mole % UF4, melting at 490°C. The LiF-ThF4 system contains four binary compounds, one (3LiF*ThF4) which melts congruently, with two eutectics at 570°C and 22 mole % ThF4 and at 560°C and 29 mole % ThF4. The ternary system LiF-ThF4-UF4 shown in Fig. 3, has no ternary compounds and a single eutectic freezing at 488°C with 1.5 mole % ThF4 and 26.5 mole % UF4. Most of the area on the diagram is occupied by the primary phase fields of the solid solutions UF4-ThF4, LiF-4UF4-LiF*4ThF4, and LiF*UF4-LiF*ThF4.Liquidus temperatures decrease generally to the LiF-UF4 edge of the diagram. The single-fluid molten-salt breeder fuel will need a concentration of ThF4 much higher than that of UF4. Accordingly, the phase behavior of the fuel parallels that of the LiF-BeF2-ThF4 system. Figure 4 gives the ternary system LiF-BeF2-ThF4; this system shows a single ternary eutectic at 47 mole % LiF and 1.5 mole % ThF4, melting at 360”C.637The system is complicated to some extent by the fact that the compound 3LiF-ThF4 can incorporate Be2+ ions in both interstitial and substitutional sites to form solid solutions whose compositional extremes are represented by the shaded triangular region near that compound. Liquidus temperatures <55OoC (1022°F) are available at ThF4 concentrations as high at 22 mole %. The maximum ThF4 concentration available at liquidus temperatures of 500°C (932°F) is above 14 mole %. Inspection of the diagram reveals that a considerable range of compositions with >10 mole % ThF4 will be completely molten at or below 500°C. .Asexpected from the general similarity of ThF, and UF4 - and especially from the substitutional behavior shown by the LiF-UF4-ThF4 system (Fig. 3) - substitution of a small quantity of UF4 for ThF4 scarcely changes the phase behavior. Accordingly and to a very good approximation, Fig. 4 represents the behavior of the LiF-BeF2-ThF4-UF4 (MSBR fuel) system over concentration regions such that the mole fraction of ThF4 is much greater than that of UF4.
11. C. F. Weaver, R. E. Thoma, H. Insley, and H. A. Friedman, “Phase Equilibria in the System UF4-ThF4 and LiF-UF4-ThF4,” J. Amer. Ceram SOC.43,213 (1960).
Fig. 3. The system LiF-ThF,-UF+
6 ORNL-LR-WG 3742OAR7
ThG l l l i
A TEMPERATURE IN OC COMPOSITION IN mole 7â€™
Fig. 4. The system LiF-BeFz-ThF4.
The success of an MSBR is strongly dependent on the compatibility of the container materials with the molten salts used in the primary and secondary circuits of the reactor. Because the products of oxidation of metals by fluoride melts are quite soluble in the corroding media, passivation is precluded, and the corrosion rate depends on other factors, including the thermodynamic driving force of the corrosion reactions. Design of a practicable system utilizing molten fluoride salts, therefore, demands the selection of salt constituents such as LiF, BeF, ,UF4, and ThF4 that are not appreciably reduced by available structural metals and alloys whose components Fe, Ni, and Cr can be in near thermodynamic equilibrium with the salt. A continuing program of experimentation over many years has been devoted to definition of the thermodynamic properties of many corrosion product species in molten LiF-BeF, solutions. Many of the data have been obtained by direct measurement of equilibrium pressures for reactions such as H,(g) + FeF,(d)
* Feo(c) + 2HF(g)
Table 2. Standard free energies of formation for species in molten 2LiF-BeF2
733 to 1000°K Material“
- a d (kcal/mole)
141.8-16.6 X 243.9-30.0 X
T°K f K
UFdd) UF4 (d) ThF4(d) ZrF4(d)
338.0-40.3 X f K 445.9-57.9 x TOK 491.2-62.4 X T°K 453.0-65.1 X lo5 f K
99.3 97.0 107.2 97.0
NiF?(d) FeFz(d) QFz(d)
146.9-36.3 X f K 154.7-21.8 X f K 171.8-21.4 X lo-’ f K
55.3 66.5 75.2
370.9-69.6 X 10” f K
“The standard state for LiF and BeF2 is the molten 2LiFsBeF2 liquid. That for MoFs(g) is the gas at 1 atm. That for all species with d is that hypothetical solution with the solute at unit mole fraction and with the activity coefficient it would have at i n f ~ t dilution. e
where g, c, and d represent gas, crystalline solid, and solute, respectively, using the molten fluoride (1) as reaction medium. Baes has reviewed all these studies’ and, by combining the data with the work of others, has tabulated thermodynamic data for many species in molten 2LiF*BeF2. Table 2 records pertinent data for the major components of MSRE and MSBR fuels and for corrosion products in molten 2LiF*BeF2. From these data one can assess the extent to which UF3-bearingmelt will disproportionate according to the reaction
For the case where the total uranium content of the salt is 0.9 mole % (as in the Molten-Salt Reactor Experiment), the activity of metallic uranium (referred to the pure metal) is near lo-’ with 1% of the UF4 converted to UF3 and is near 2 X lo-’ with 20% of the UF4 so converted.” Operation of the reactor with a small fraction (usually <2%) of the uranium present as UF3 is advantageous insofar as corrosion and the consequences of fission are concerned. Such operation with some UF3 present should result in formation of an extremely dilute (and experimentally undetectable) alloy of uranium with the surface of the container metal. Operation with >SO% of the uranium as UF3 would lead to much more concentrated (and highly deleterious) alloying and to formation of uranium carbides. All evidence to date demonstrates that operation with relatively little UF3 is completely satisfactory.
METAL CORROSION The data of Table 2 reveal clearly that in reactions with structural metals (M) 2UF4(d)
+ M(c) + 2UF3(d) + MF,(d),
chromium is much more readily attacked than iron, nickel, or molybdenum.13J4 12. C. F. Baes, Jr., ‘The Chemistry and Thermodynamics of Molten Salt Reactor Fuels,” presented at AIME Nuclear Fuel Reprocessing Symposium at Ames Laboratory, Ames, Iowa, Aug. 25,1969. Published in the 1969 Nuclear Metallurgy Symposium,Vol. 15, by the USAEC Division of Technical Information Extension. 13. G. Long, Reactor Chem Diu. Annu. Progr. Rep. Jan. 31,1965, ORNL-3789, p. 65. 14. J. W. Koger, MSR Program Semiannu. Progr. Rep. Aug. 31,197O,ORNL-4622, p. 170.
Nickel-base alloys, more specifically Hastelloy N and its modifications, are considered the most promising for use in molten salts and have received most attention. Stainless steels, having more chromium than Hastelloy N, are more susceptible to corrosion by fluoride melts but can be considered for some applications. Oxidation and selective attack may also result from impurities in the melt,
M + NiF,
MF2 + Ni,
M + W F + M F , +H2, or oxide films on the metal, NiO + BeF,
followed by reaction of NiF, with M. Reactions (8), (9), and (10) will proceed essentially to completion at all temperatures within the MSBR circuit. Accordingly, such reactions can lead (if the system is poorly cleaned) to a rapid initial corrosion rate. However, these reactions do not give a sustained corrosive attack. Reaction (7) with UF4, on the other hand, may have an equilibrium constant which is strongly temperature dependent; hence, when the salt is forced to circulate through a temperature gradient, a possible mechanism exists for mass transfer and continued attack. Reaction (7) is of significance mainly in the case of alloys containing relatively large amounts of chromium. If nickel, iron, and molybdenum are assumed to form regular or ideal solid solutions with chromium (as is approximately true), and if the circulation rate is very rapid, the corrosion process for alloys in fluoride salts can be simply described. At high flow rates, uniform concentrations of UF3 and CrF2 are maintained throughout the fluid circuit. Under these conditions, there exists some temperature (intermediate between the maximum and minimum temperatures of the circuit) at which the initial chromium concentration of the structural metal is at equilibrium with the fused salt. This temperature T Bis~called the balance point. Since the equilibrium constant for the chemical reaction with chromium increases with increasing temperature, the chromium concentration in the alloy surface tends to decrease at temperatures higher than T B and ~ tends to increase at temperatures lower than T B ~At. some point in time, the dissolution process will be controlled by the solid state diffusion rate of chromium from the matrix to the surface of the alloy. In some melts (NaF-LiF-KF-UF4, for example) the equilibrium constant for reaction (7) with chromium changes sufficiently as a function of temperature to cause formation of dendritic chromium crystals in the cold zone. For MSBR fuel and other LiF-BeF2-UF4 mixtures, the temperature dependence of the mass transfer reaction is small, and the equilibrium is satisfied at reactor temperature conditions without the formation of crystalline chromium. Thus, the rate of chromium removal from the salt stream by deposition at cold-fluid regions is controlled by the rate at which chromium diffuses into the cold-fluid wall; the chromium concentration gradient tends to be small, and the resulting corrosion is well within tolerable limits. A schematic of the temperature gradient mass transfer process is shown in Fig. 5.
DIFFUS I ON TO SURFACE -
SOLUTE ESCAPE THROUGH NEAR-SURFACE LIQUID LAYER
DIFFUSION INTO ill% LIQUID
TRANSPORT TO COLD PORTION OF SYSTEM
SUPERSATURATION - ___ -NUCLEATION o GROWTH TO STABLE CRYSTAL SlZE X
- - - -
SUPERSATURATION AND DIFFUSION - THROUGH LIQUID
NUCLEATION AND GROWTH ON METALLIC WALL OR DIFFUSION INTO WALL
- - - - -
Fig. 5. Temperature-gradientmass transfer.
SALT PREPARATION The salt for the loops was prepared by the Fluoride Processing Group of the Reactor Chemistry Division. Although starting materials of very high purity were used in production of fused fluoride mixtures, further purification was needed before the salts were used in loop systems. Two steps were required: one for the removal of oxides and sulfides and one for the removal of metallic fluorides. For the blanket and fuel salts, the oxides and sulfides were removed by gas sparging for several hours (usually 10 to 20) at 650째C with an anhydrous mixture of HF in hydrogen (1:4). The purification reactions are of the
-.type 02- + 2HF
* 2F- + H2O.
The process is continued until the same amount of HF leaves the reaction vessel as enters. The reaction is then considered complete. Gas sparging of the melt at 70O0Cwith hydrogen alone for several hours (usually 20 to 40) was used as the final phase of the purification process to reduce FeF, and NiF2 concentrations to low values and to remove any residual HF:
H2 +MF, *Mo + W F .
10 The reduction of CrF, by hydrogen is too slow to be effective at process temperatures. However, the chromium concentration of the starting materials is very low. The by-product of the hydrogen sparging is HF, and the process is continued until the HF evolution is below a certain level.
MATERIALS SELECTION AND FABRICATION The Hastelloy N material for loops 15, 16, 18, 19, and 21 was from heat No. 5097 obtained from Stellite Division, Cabot Corp, and the composition is given in Table 3. The loops were fabricated from 0.750-in-OD annealed tubing with a wall thickness of 0.072 in. Machined pieces were annealed at 1175째C in Hz before welding. The material was TIG welded in conformance with ORNL Specifications PS-23 and PS-25 and inspected under ORNL Specification MET-WR-200. After welding, the loops were stress relieved at 880째C for 8 hr. Table 3. Composition of Hastelloy N loop material (heat 5097) Element
The loops were heated by pairs of clamshell heaters placed end to end around two legs of the loop (Fig. 1). The input power was controlled by silicon controlled rectifier (SCR) units, and the temperature controlled by a current proportioning controller. The loop temperatures were measured by Chromel-P vs Alumel thermocouples that had been spot welded to the outside of the tubing, covered by a layer of quartz tape, and then covered with stainless steel shim stock. Tubular electric heaters controlled by variable autotransformers furnished the heat to the cold leg portions of the loops during startup of the loops. Before filling with salt, the loops were degreased with ethyl alcohol, dried, and then heated to 150째C under vacuum to remove any traces of moisture. A helium mass spectrometer leak detector was used to check for leaks in the system. The procedure for filling the loops consisted of heating the loop, the salt pot, and all connecting lines to approximately 550째C and applying helium pressure to the salt supply,vessel to force the salt into the loop. Air was continuously blown on freeze valves leading to the dump and flush tanks to provide a positive salt seal. Normally the first charge of salt was held for 24 hr in the loops at the maximum operating temperature and then dumped. This flush salt charge was intended to remove surface oxides or other impurities left in the loops. The loop was then refilled with fresh salt, and operation began. Once the loop was filled, the heaters on the cold leg of the loop were turned off. As much insulation was removed as necessary to obtain the proper temperature difference by exposing the cold leg to ambient air. Helium cover gas of 99.998% purity and under slight pressure (approx 5 psig) was maintained over the salt in the loops during operation.
With the exception of loop 1258 which only had specimens in the hot leg, the loops all contained 14 to 16 specimens 0.75 X 0.38 X 0.030 in., each with a surface area of 0.55 in.' (3.45 cm'). Generally two of the specimens were titanium-modified Hastelloy N. (Modifications to the standard Hastelloy N composition were made to test for improved mechanical properties after neutron irradiation.) The composition of the standard and modified Hastelloy N specimens is given in Table 4. Eight specimens were attached at different vertical positions on each of two 'I8-in. rods. One rod was inserted in the hot leg and another in the cold leg. The rods were placed into or removed from the loop from standpipes atop each leg. The rods were moved through a Teflon sliding seal compression fitting at the top of the standpipe and a ball valve at the bottom. Another ball valve on the loop above each leg assured removal or insertion without disturbing loop operation or introducing air contamination. The corrosion specimens were withdrawn periodically along with salt samples to follow corrosion processes as a function of time. During the removal periods all specimens were weighed and measured. .Portions of the hottest and coldest specimens were removed and examined metallographically during tests, and all specimens were examined metallographically after test. Table 4. Compositionof Hastelloy N specimens Weight percent
Mo Ti-modified 13.8 Standard 17.2
RESULTS Hastelloy N
Loop 15. Loop 15 was operated to determine the compatibility of a proposed blanket salt for a two-fluid molten salt breeder reactor with Hastelloy N. Figure 6 shows loop 15 on the left in place befole operation. For loop 15 the fuel pot and associated lines had to be heated to 730째C and hiher than normal inert gas pressure applied to fill the loop with salt. During the initial salt transfer the fill line failed and resulted in a spill. After repairs, we managed to fdl the loop with the flush charge but found it impossible to initiate circulation even after heating the loop's hot leg to 760째C. The loop was drained and then refilled with clean salt and put into operation. The loop was operated at a maximum temperature of 676째C with a temperature difference of 54OC. A helium cover gas under slight positive pressure (-5 psig) was maintained over the salt in the loops during operation. On May 1, 1968, after 2003 hr of uneventful operation, the loop cooled due to a blown fuse, and all salt was frozen. Heat was applied to the loop in order to thaw the salt, and a rupture occurred in the hot leg loop piping 30 in. down from the hot leg surge tank (Figs. 7 and 9, thus ending the operation of loop 15. The weight changes of the specimens in the hottest and coldest positions are plotted vs time of operation in Fig. 9. The standard Hastelloy N specimen at a lower temperature lost more weight than the titanium-modified specimen at the higher temperature. We attribute this increased corrosion resistance to the lower iron concentration of the titanium-modified alloy (Table 4). Weight losses were measured for hot leg specimens and weight gains for cold leg specimens, thus implying that temperature gradient mass transfer had occurred. The weight changes in all cases were quite small.
Fig. 7. View of loop 15 and the ruptured area of NCG15.
2 Ti MODIFIED HASTELLOY N A STANDARD HASTELLOY N 0
g o a
Fig. 9. Weight changes of Hastelloy N specimensin loop 15 vs time of operation in LiF-BeFz-ThF4(73-2-25 mole %).
Figure 10 shows microstructures of the specimens in the hottest and coldest positions, respectively. There is little or no indication of corrosion or mass transfer effects. The salt was periodically analyzed â‚Źor its major constituents, the major alloying elements of the container material, and oxygen and water. The chromium and iron increased with time, but the changes were very small (about 20 ppm increase). Nickel showed a small overall increase, molybdenum remained at <20 ppm during operation, oxygen ranged from <50 to a high of 244 to a value of 75 ppm just before the rupture, and water was <500 ppm in each analysis. The latter four values are quite low and preclude any possibility of air or water contamination. Table 5 gives pertinent details of loops that had operated in past years for various times with LiF-ThF4 (71-29 mole %) salt. The two Inconei loops that operated for a year (8760 hr) showed subsurface void formation for distances up to 6'1'~mils,but the INOR-8(Hastelloy N) loop that operated for a year showed no voids. The improved behavior of INOR-8 was somewhat expected since there is less chromium present. None of the loops showed any signs of plugging, and no large increases of any of the alloy constituents are noted in the salt. Our experiment substantiated and quantified the previously observed good behavior of Hastelloy N in LiF-ThF4 salts. From the operational viewpoint, this salt provided more difficulties than any other fluoride salt that has been handled by the present Reactor Materials Group personnel. The first problem was the high temperature (730Â°C) needed to transfer the fuel and the apparent presence of unmelted salt constituents. It is thought that there was perhaps a separation of a high melting component which caused this problem. The second problem was the rupture of the loop while trying to thaw the frozen salt. This thawing procedure had been used with other salts quite successfully with no failures. Loop 15A. The ruptured area of loop 15, which still contained frozen salt, was cut from the loop and another piece of tubing was attached by means of compression-type fittings. The loop was then heated, the salt was melted and dumped, and the test specimens were removed. The temporary fitting was removed, and the joints to be welded were reamed to remove any remaining salt and corroded metal and filed to provide the proper weld joint configuration. Welding was done in conformance with ORNL specifications
. Fig. 10. Microstructures of HasteUoy N specimens for loop 15 after 2000 lu exposure to LiF-BeFz-ThF4 (73-2-25 mole 46). (u) Hot leg, 676OC; (b) cold leg, 613OC.
Table 5. Thermal convection loops that operated with LiF-ThF4 (71-29 mole %) salt
Maximum temperature (“C)
Chemical changes insalt @pm) Cr
Hot leg condition
11 1 75
INOR-8b INOR-8‘ INOR@
8760 3114 io00
733 690 682
93 72 61
240 65 40
60 50 120
Light surface roughening, few voids to a depth of <1 mil. Few pits to l’h mils, few voids to a depth of <1 mil. Moderate surface roughening. Intergranular voids to 6% mils. Moderate surface roughening Pits to 1 mil, voids to 5 mils. Moderate surface roughening Heavy surface roughening. Lightsurfaceroughening. Light surface roughening.
‘15 Cr, 7 Fe, bal Ni. b17Mo,8 a,5 Fe, bal Ni. ‘15 Mo, 6 0 . 5 Fe, bal Ni. %.8 Mo, 6.99 Cr, 4.85 Fe, bal Ni. i
PS-23 and PS-25 and inspected under ORNL specification MET-WR-200. The first welding attempt was unsuccessful because of poor penetration from excessive gas pressure in the loop. The second attempt was successful and demonstrates that a successful weld can be made on material that has contained a molten salt. The loop was filled with salt from the original batch and designated 15A. After operation began, specimens were found to have a “glaze” or coating (probably a high-melting thorium compound) that was impossible to remove without damaging the specimen. However, based on changes of chromium concentration and metallographic studies, little if any mass transfer was indicated. Toward the end of the run the coating on specimen surfaces disappeared, and the weight changes were measurable. For a total specimen exposure time of 37,792 hr, the maximum weight loss was 4.7 mg/cm2 ,equivalent to a uniform corrosion rate of 0.05 mil/year, and the maximum weight gain was 4.2 mg/cm2. Figure 11 shows the microstructure of the hottest and coldest specimens. Some attack along the grain boundaries of the hottest
specimen is seen. Loop 18 and 19. Loops 18 and 19 were constructed of standard Hastelloy N with removable specimens in each leg and were operated with the salt mixture 68% LiF-20% BeF2-1 1.7% ThF4-0.3% UF4 (mole %). Loop 19 had a molybdenum hot finger containing bismuth at the bottom of the hot leg (Fig. 12) which allowed contact between the flowing salt and the bismuth. The loops were operated to obtain data on the compatibility of a fertile-fissile salt mixture witF Hastelloy N and to determine if contacting the salt with liquid bismuth would affect the corrosion rate. After a power outage at 4741 hr the bismuth finger on loop 19 was inadvertently heated to temperatures over 1000°C. Subsequent examination disclosed localized melting of the Hastelloy N which surrounded the molybdenum container. Portions of the loop and the finger were removed for examination and replacement parts fabricated for repair. Prior to the 4741-hr shutdown the maximum weight loss for a standard Hastelloy N specimen at 704°C was 0.8 mplcrn?. Assuming uniform dissolution this weight loss is equivalent to 0.07 mil/year, an insignificant corrosion rate. The chromium content of the salt increased from 25 to 66 ppm while iron decreased from 78 to 23. Figure 13 shows the metallographic appearance of the hottest and coldest
Fig. 11. Microstructures of Hastelloy N specimens from loop 15A after 37,792 hr exposure to LiF-BeFz-ThF4 (73-2-25 mole 5%). (a) Hot leg, 676OC; ( b ) cold leg, 613OC. SOOX.
Bismuth â€œhot fiigerâ€? contained in molybdenumwith Hastelloy N jacket on loop 19.
. Fig. 13. Microstructure of Wastelloy N from loop 19 exposed to LiF-BeF2-ThF4-UF4 (68-20-11.7-0.3 mole %) 4741 hr. (a) Hot leg, 700OC; ( b ) cold leg, 550째C.
specimens. Little attack or depo&ion is seen. The bismuth content of the salt was <20 ppm for the last 1500 hr. After the temperature excursion the salt and the bismuth at the top of the finger were both analyzed for certain metal impurities, and the results are given in Table 6. Table 6 shows that bismuth extracted impurities from the salt in quantities proportional to the solubility of these structural metals in bismuth. Analysis of the dumped salt from loop 19 disclosed 225 ppm bismuth. At the time of this analysis, in loop 18 the maximum weight loss of a standard Hastelloy N specimen was 0.8 mg/cm2 at 704OC in 3400 hr, a very low rate, equivalent to 0.08 mil/year assuming uniform attack. The chromium concentration in the salt in this loop had increased from 21 to 90 ppm. We showed no difference in mass transfer in the two loops at this time. The specimen from the hottest position of loop 19 was bent around a ‘&-in.diam tube and examined metallographically (Fig. 14). There was no indication of cracking or weakening of grain boundaries, and there were no signs of salt or bismuth attack, Table 6. Analysis of salt and bismuth from hot finger portion of loop 19 Major constituent
Fe Mo Bi
10 0.2 225
Solubility at 60O0@ 6.0% 140 ppm 50 PPm <1 PPm
%. J. Klamut et al., “Material and Fuel Technology for an LMFR,” pp. 433-72 in Rogress in Nuclear Energy, Series IV, vol. 2, Technology, Engineeringand Safety, Pexgamon, London, 1960.
Fig. 14. Microstructure of stressed Hastelloy N specimen from loop 19 exposed to LiF-BeFz-ThF4-UF4 (68-2G11.7-0.3 mole 4%) for 4741 hr at 7OOoC.
Repairs were made to loop 19 and the molybdenum finger, and the system was restarted with fresh salt and bismuth with the loop designated as 19A. Loop 19A operated 24,515 hr, and the weight changes are shown in Fig. 15. Little if any attack was seen on the hottest specimen. Assuming uniform loss the maximum weight loss was equivalent to only 0.02 mil/year. A modified Hastelloy N alloy (Ni-13.0% Mo-8.5% Cr-0.1% Fe-LT.8% Ti-1.6% Nb) lost less weight than a standard alloy at the same position. We attribute this difference to the low iron in the modified alloy, compared with about 5% in the standard alloy. The 'chr6miu1h content of the salt increased ,194 ppm in 18,000 hr, while iron decreased 70 ppm, and there was no detectable bismuth in the &:During the last exposure period, the specimens in the hot leg were inadvertently$placed4 in.,lower than usual. This put the bottom specimen into the molten bismuth during operation. On removing the stringer, this bottom specimen was missing. The end of the stringer appeared Po have $been.in-contactwith the bismuth but was not dissolved. Thus it is likely that the very small specimen attachment ,pins dissolved during'the run, and the specimen fell off the stringer. As we had surmised earlier in loop 19, the bismuth in contact with the salt appeared to have had no effect on our mass transfer results as loops 18 and 19 sho e amount of mass transfer (Fig. 16). Loop 18 operated a total of 15,93 maximum weight loss was 1.5 mg/cm' at 704'C, equivalent to a corrosion rate of 0.05 um in the salt increased from 20 to 190 ppm while iron decreased from 80 t
, ORNL-DWG 74-699013
OPERATING TIME (hr) I
Fig. 15. Weight changes of Hastelloy N fram loop 19 exposed toLiF-BeFz-ThF4-UF4(68-20-11.7-0.3 mole %) for various times. ORNL-DWG f0-4934R
z o a
5 -2 -3
2000 3000 OPERATING TIME (hr)
of Hastelloy N in LiF-BeF2-UF4-ThF4salt with and withou
Loop 21. Loop 21, a Hastelloy N thermal convection loop (Fig. 17) with removable specimens in each leg and containing the Molten-Salt Reactor Experiment reference fuel salt (Table l), operated for 13,798 hr. The loop was equipped with electrochemical probes which measured the U3+/U4+ ratio, and hence provided an instantaneous measure of the oxidation potential of the salt. The probes were designed and operated by J. M. Dale and A. S. Meyer of the Analytical Chemistry Division. Previous use of these probes had been limited to small static systems, and this experiment was intended to evaluate their possible use for on-stream analysis in a large system. This loop differed from our other thermal convection loops in that the salt flow up the hot leg went directly into a large surge tank. In our other loops the salt was circulated only through tubing which was in a harp-shaped configuration. From the large surge tank the salt then flowed out the bottom of the tank into a crossover leg and into the cold leg. The electrochemical probes passed through mechanical fittings (separated from the metal by Teflon), which were on risers 10 in. from the surge tank (to protect the Teflon from the heat of the salt) and then entered the salt in the large hot leg surge tank, as shown in Fig. 18. There were five access ports for the probes. The loop was filled on July 20, 1971, and held under isothermal conditions at about 65OoC until July 26, at which time the cold leg temperature was established and Hastelloy N specimens were inserted into both the hot and cold leg of the loop for corrosion studies, Analyses of the U3+concentration of the melt were started on July 22 and were continued on a routine basis until the specimens were removed from the loop on August 23. More details about these analyses can be found in refs. 15, 16, and 17. The original measurements in the melt indicated that about 0.02% of the total uranium was present as U3+.The U* concentration showed a gradual increase until a value of 0.05%was reached at 475 hr of loop operation. At this point the rate of formation of U3+increased, and the concentration reached a value of about 0.15% when the metal specimens were removed from the loop. The maximum weight loss of a hot leg specimen was 012 mg/cm2,and the maximum weight gain of a cold leg specimen was 0.05 mg/cm2. To evaluate whether material floating on the salt was affecting the potential measurements, the electrode assembly was modified to allow the salt to be flushed from around the electrode with helium. This assembly was installed in the loop after the metal specimens were removed. The electrode was encased in a '/?-in. nickel tube, open at the bottom, which protruded below the surface of the melt. During computer-controlled runs the salt entered the electrode compartment from below the melt surface and remained there for the time of measurement. The salt was then flushed from the compartment, and the electrode remained in a helium gas envelope when not in use. This appeared to keep floating material away from the electrode and also should have increased the lifetime of the electrodes or electrode area-defining insulators which may be added at a later time. After the system was started the analyses were performed unattended through computer control. At initiation of the analyses a signal from a logic circuit that we added to the computer started a timer which caused the pressure in the electrode assembly to be released, and salt entered the electrode compartment. The computer then operated the voltammeter t tm five analyses for Us, and the results plus some diagnostic information Were printed out on a Te fter each analysis. At the end of the run the average U3+concentration and standard deviation were ed and printed out. When the run was completed, the timer shut off causing the salt to be flushed from the electrode assembly. As an example of the precision of the analysis system, a standard deviation of 2.1% was obtained for the results of the hourly analyses made over a one-weekend period when the U3+concentration appeared to be relatively stable. -~~
15. J. M.Dale and T. R.Mueller,MSR Program Semiannu. Progr. Rep. Feb. 28,1971,0RNL4676,p. 138. 16. J. M. Dale and A. S. Meyer,MSR Program Setmannu. Rogr. Rep. Aug. 31,1971, ORNL4728,pp. 69-70. 17. J. M. Dale and A. S. Meyer, MSR Program Semiannu. Progr. Rep. Feb. 29,1972, ORNL4782,pp. 77-79.
6 8 - 3987R3
1: I I I !I.
I I ~
Fig. 17. Schematic of loop 21.
Fig. 18. Upper portion of loop 21.
The percent of the total uranium which was present as U* for the first 3600 hr of loop operation is shown in Figs. 19-21. The irregular appearance of the data at 600 hr was due to large temperature fluctuations in the electrode tank. The first measurements with the shielded electrode were made at 1200 hr and are plotted as the squares in Figs. 19 and 20. At about 1250 hr it was first noted that analyses with the shielded and unshielded electrodes gave different values of the U3+concentration. This was later shown to be an effect of the nickel tube around the shielded electrode and not to a difference in the electrode response. At 2350 hr the nickel tube shield was raised out of the melt, and the measurements with the two electrodes were in agreement as shown in Fig. 20. The second time the specimens were removed was November 29, 1971. The specimens had been exposed a total of 2513 hr, and the maximum weight loss was 0.2 mg/cm2 while the maximum weight gain was 0.05 mg/cm2. The last time the specimens were removed was February 8, 1972. The total exposure time was 4169 hr, and the maximum weight loss was 0.23 mg/cm2, which would correspond to a corrosion
ORNL- DWG. 71-14377R
& + '
Fig. 19. Uranium@) in loop 21 fuel salt, 7/20/71 to 9/8/71.
ORNL-DWG. 74- 14378R
3 + 0.20, lo3 I
Fig. 20. Uranium(TI1)in loop 21 fuel salt, 9/8/71 to 10/28/71.
27 ORNL-DWG. 71-+4379R
3200 LOOP OPERATION , hours
Fig. 21. Uranium(lI1) in loop 21 fuel salt, f0/28/71 to 12/17/71.
rate of 0.02 mil/year, assuming uniform material removal. The chromium content of the salt increased 40 ppm Except for the first time, when the U3+concentration was already at a low value, the insertion of the metal specimens appeared to introduce an oxidant which caused a decrease in the U* concentration (1316 hr on Fig. 20 and 3200 hr on Fig. 21). Special precautions were taken for the next specimen insertion to determine if this operation could be performed without oxidizing the U*. At 1725 hr the shielded electrode, which had previously been removed for examination, was put back into the loop without immersing it into the salt. As shown in Fig. 20,the U3+concentration decreased and then rapidly recovered, probably due to dilution effects caused by the salt flow. In summary, the results of the ratio measurements generally showed excellent reproducibility and were consistent with the known factors of loop operation. Despite certain operational problems such as the offset in the potential of shielded electrodes, smaller offset voltages observed between the reference and working electrodes, and the establishment of accurate calibrations for the determination of corrosion products, experience with this test system gives confidence that this relatively simple transducer system can be widely applied to other test systems and ultimately to in-line reactor streams. Loop 16A. Loop 16A was operated to determine the kinetics of tellurium transport in a temperature gradient loop system where the tellurium is introduced as a metallic coating on Hastelloy N. The reason for the experiment was the discovery of cracks in stressed Hastelloy N that had been exposed to fuel salt in the MSRE,' * and subsequent evidence that tellurium entering salt as a fission product could cause cracks of this nature. The test bed for this experiment was a Hastelloy N thermal convection loop that had previously operated -38,000 hr as loop 16A with the fuel mixture 65.5% LiF-34% BeF2-0.5% UF4 (mole %). Operating conditions for loop 16A are noted in Table 1. For the initial experiment (which lasted 3400 hr), a Hastelloy N specimen coated with 1.6 mg/cm2 tellurium was added to the normal complement of standard Hastelloy N specimens. In the first 1300 hr of operation the weight loss of the tellurium-coated specimen equaled the amount of tellurium coated on the specimen. In the last 2100 hr the weight loss of the tellurium-coated specimen was the same as the hottest 18. H. E. McCoy and B. McNabb, Intergranular Czacking of INOR-8in the MSRE,ORNL-4829 (November 1972).
Hastelloy N specimen located in a neighboring position at the same temperature. Thus, all the tellurium was apparently removed in the first 1300 hr. Half the tellurium removed was found in the salt and half on a specimen in the cold leg. These results indicate that tellurium has some solubility in the salt and is capable of being redistributed by temperature-dependent mass transfer. The specimens were removed from the loop and were stressed and examined metallographically for cracks. No cracks were found. We then placed radioactive tellurium-coated Hastelloy N specimens in the hot and cold leg of the loop and we used weight change measurements and radioactive analysis to monitor the movement of the tellurium. The isotope used was 27mTe,and it was electroplated on the specimens. Specimens were placed in the vapor space, in stagnant salt, and in the circulating salt of the loop. The specimens were removed after 42, 159, 396, 701, 1318, and 1792 hr exposures. We expected no corrosion of the Hastelloy N by the fuel salt in these time periods, so all weight changes were attributed to movement of the tellurium. After the first 42 hr in the loop, all specimens lost at least 66% of their initial activity. Our standard specimen which had remained at room temperature in air lost 4% of its activity. After 159 hr in the loop, all specimens had lost 75% of their initial activity. The standard specimen had lost 8%.In the next two weighmg and measuring periods, we saw an increase of activity on the cold leg specimens and a continued decrease of activity on the hot leg specimens. In the last two examination periods, there were almost no weight or activity changes. Weight changes correlated quite well with the activity measurements; specimens in the hot leg lost weight, and specimens in the cold leg gained weight. Therefore, after large initial activity losses, we observed mass transfer of tellurium from the hot leg to the cold leg analogous to our normal movement of chromium in a Hastelloy N-salt system. In a Hastelloy N system, until an equilibrium between the salt and the alloy is established at one point in the system, all points of the loop lose material. After this equilibrium is established at the balance point, losses are seen in the hot leg accompanied by gains in the cold leg. The tellurium in this system behaved in somewhat the same manner.
Type 304L Stainless Steel Loop 1258. Loop 1258, constructed of type 304L stainless steel (1 1.07% Ni, 18.31 % Cr, 0.028% C, bal Fe) and containing removable corrosion specimens in the hot leg, operated nine years (80,000hr) and thus provided long-term stainless steel-fuel salt compatibility data. An LiF-BeF2-ZrF4-UF4-ThF, (70-23-5-1-1 mole %) salt circulated in the loop at a maximum temperature of 688OC and a minimum temperature of 588OC. The loop with its one surge tank is seen in Fig. 22. Corrosion specimens were present in the hot leg only. The loop was started July 29, 1963. Four of ten specimens were removed October 31, 1963, after 2244 hr exposure and are pictured in Fig. 23. The weight losses were 11.6, 11.3,8.1, and 3.3 mg/cm2. In terms of uniform material removal, the maximum corrosion rate was over 2 mils/year. Figure 24 shows a micrograph of a specimen removed after 15,000 hr at 68OoC. We see a maximum of 2 m i l s grain boundary penetration. In January 1967 after approx 30,000 hr, the remainder of the original specimen set was removed, and a second set, consisting of ten new specimens, was placed in the hot leg. The hottest specimen was replaced after 3700 hr, and the rest of the specimens remained in the loop (periodic removals for examination) until its shutdown. The specimen exposed at the highest temperature, 688"C, was removed for detailed metallurgical analysis after 5700 hr (between May 1967 and February 1968). Figure 25 shows all the specimens at this time (9400 hr exposure). No gross corrosive effects are evident. The microstructure of the hottest specimen is seen in Fig. 26. Voids extend into the matrix for a maximum distance of 2.5 mils along grain boundaries. The microprobe analysis of this specimen for chromium and iron is shown in Fig. 27. Note that the chromium concentration of the alloy is decreased for a distance of 28 pm. Thus chromium depletion does appear to be occurring in this system. '
Fig. 22. Loop 1258.
Fig. 23. First corrosion specimens in loop 1258.
Fig. 24. Microstructure of type 304L stainless steel specimen exposed to LiF-BeFz-ZrF4-ThF4-UF4(7@23-5-1-1mole %) for 15,000 hr at 68OoC.
. . - . - ' ' * ' i PHOTO
Fig. 25. Type 304L stainless steel specimens from loop 1258 exposed to LiF-BeFz-ZrF4-ThF4-UF4(70-23-5-1-1 mole
, w I
46) for 9400 hr at temperature ranges from 688OC (top specimen) to 668OC (bottom specimen).
32 After 62,600 hr operation of the loop (September 1970) we replaced the heaters and thermocouples of the loop. Operation of the loop had become increasingly difficult as heater and thermocouple failures became more frequent. When the heaters were removed, we found many green chromium oxide crystals on the loop exterior directly under the heaters. These crystals were the result of a fairly common phenomenon in Nichrome-wound heaters where chromium, because of its high vapor pressure, is selectively vaporized from the heater wire over a long period of time. This vaporization changes the heating characteristics of the
Fig. 26. Microstructure of type 304L stainless steel specimen for loop 1258 exposed to LiF-BeF+F4-ThF&F4 (70-23-5-1-1mole %) for 5700 hr at 688째C. ORNL-DWG 72-1121
$ 60 c
Fig. 27. Chromium and iron concentrationgradient in a typei304L stainless steel specimen from loop 1258 exposed to LiF-BeF&rF4-ThF4-UF4 (70-23-5-1-1mole %) for 5700 hr at 688째C.
wire and certainly contributed to some of our operating problems. The salt was successfully thawed and loop operation continued. The weight changes of the second specimen set after 32,000 hr are seen in Fig. 28. Note the dependence of weight loss with time and temperature. The microstructures of three specimens after 45,724 hr salt exposure are shown in Fig. 29. Voids extend for at least 10 m i l s into each specimen. At loop shutdown the second specimen set had been exposed to the salt for 49,057 hr. The maximum weight loss was 95.9 mg/cm2, equivalent to a uniform corrosion rate of 0.86 mil/year. For both specimen sets, the weight losses and depth of void formation increased approximately in proportion to the one-half power of the operating time. This suggests that the corrosion process was selective toward chromium and was controlled by the solid-state diffusion rate of chromium.
Maraging Steel Because of interest in iron-base alloys with lower chromium contents for possible containment of molten salts, we tested a maraging steel (12% Ni-5% Cr-3% Mo-bal Fe) specimen in loop 1258. The specimen was annealed 1 hr at 800째C and air cooled. Table 7 compares the weight loss and corrosion rate of this specimen with type 304 stainless steel and Hastelloy N under similar conditions of exposure. As expected, the maraging steel showed better corrosion resistance than the stainless steel because of its lower chromium content. However, the corrosion behavior of the Hastelloy N was still superior to both. Figure 30 shows the metallographic appearance of the maraging steel specimen after exposure for 5700 hr at 662째C. Most of the attack is manifested as surface pitting, but there are also subsurface voids such as were seen in the stainless steel specimens of this loop. The void formation is attributed to removal of chromium atoms from the surface. This results in a concentration gradient and causes like atoms from the underlying region to diffuse toward the surface, thus leaving behind a zone enriched with vacancies. In time these vacancies accumulate and form visible voids. The specimen of maraging steel was examined using the electron-beam microprobe.'9 Using an accelerating voltage of 20 kV and specimen current of 0.01 PA, x-ray intensities were recorded (Fe Ka,Ni Ka, Cr Ka, and Mo La) in both as-received and corroded specimens. Since x-ray intensities of a given element are directly related to the weight percent of the element, a comparison of intensities should reflect the change in composition in the attacked zone in the corrosion specimen. Table 8 shows the comparison for each of the four elements. Figure 31 shows the cathode ray tube display and corroborates the - quantitative data. One can see the depletion of iron and chromium and the increase in nickel. Molybdenum seems to remain about the same. 19.
Microprobe examination made by R. S. Crouse, H. Mateer, and T. J. Henson, Metals and Ceramics Division. Table 7. Comparison of weight losses of alloysat approx 663째C in Similar flow fuel salts in a temperature gradient system
Type 304 stainless steel Hastelloy N
Weight loss (mg/cm2) 3130 hr
3.0 6.5 0.4
4.8 10.0 0.6
Average corrosion rate (milslyear) 0.55 1.1 0.06
14 16 18 20 SPECIMEN TIME IN SYSTEM (loo0 hr)
Fig. 28. Weight changes of type 304L stainless steel specimensfrom loop 1258 exposed to LiF-BeFz-ZrF4-ThF4-UF4 (70-23-5-1-1mole %) for various times and temperatures.
Fig. 29. Microstructures of type 304L'stainlesssteel specimens from loop 1258 exposed to LiF-BeF2-ZrF4-ThF4-UF4 (70-23-5-1-1 mole %) for 45,724 hr at (a) 68S째C, (b)679OC, and (e) 674째C. Reduced 28%.
Fig. 30. Microstructure of a maraging steel (12%Ni-546 Cr-3% Mo-bal Fe) exposed to LiF-BeFz-ZrF4-ThF4-UF4 (70-23-5-1-1 mole %) for 5700 hr at 662OC. As polished.
Table 8. X-rayintensities of constituentsof maraging steel Element Fe Ni
intensity ratios, attack/as received 0.77 3.25 0.32 1.oo
Type 316 Stainless Steel Loop 22, Loop 22 was a type 316 stainless steel thermal convection loop which operated for 4491 hr with a LiF-BeFz-ThF4-UF4 salt mixture identified in Table 1.The harp portion of the loop was l-in.-OD tubing with 0.109-in. wall thickness. The material was from heat X-22662,U.S. National Tube, and the ORNL Inspection Engineering Number was IR-9141,Y-12No. 8194.The nominal composition of the alloy was 16.6% Cr, 13.6% Ni, 2.25% Mo, bal Fe. The loop was operated to determine the compatibility of stainless steel with a well-purified fuel salt. The weight chbnges of the specimens as a function of position and temperature are given in Fig. 32. Figure 33 shows the microstructure of the hottest specimen after 1410 hr. Subsurface voids are seen for a distance of 1 mil. After 2842 hr exposure the specimen at 650Â°C had lost a total of 6.2 mdcrnâ€™, equivalent to a uniform corrosion rate of 0.96 mil/year.
X-RAYS (MAG. SOOX)
Fig. 31. Characterizationof attack zone in maraging steel. Reduced 10%.
t Lt W 1000 g w I-
40 50 80 DISTANCE (in.)
Fig. 32. Weight changes of type 316 stainless steel specimens in loop 22 exposed to LiF-BeF2-ThF4-UF4 (68-20-1 1.7-0.3 mole %) as a function of position and temperature.
Fig. 33. Microstructure of type 316 stainless steel specimen in loop 22 exposed to LiF-BeF2-ThF4-UF4 (68-20-11.7-0.3 mole %) after 1410 ht at 65OoC. SOOX. I
The main corrosion reaction in this system is 2UF4 + Cr + CrFz + 2UF3 ;thus, in order to determine if we could decrease the mass transfer of the stainless steel, we added UF3 to the salt after the 2842-hr exposure measurements to make the salt less oxidizing. In the next 645-hr time period the mass transfer was somewhat less, and the overall corrosion rate was 0.83 mil/year. In the final 811-hr time period, the weight loss of the hottest specimen increased such that the uniform corrosion rate was >1 mil/year. However, the overall mass transfer, as evidenced by weight changes of other corrosion specimens, remained quite low. The average uniform corrosion rate for the hottest specimen was 1 mil/year for the entire 4298-hr period of loop operation. Figure 34 shows the microstructures of hottest and coldest specimens at the end of the run. Figure 34a shows a lOOX cross section of the specimen with voids extending about 1 mil into
the surface. Figures 34b and 34c are 500X views as polished and etched respectively. In Fig. 34c note that the etching reveals a 3-mil-wide affected area. This complete area is probably depleted of chromium. Figure 34d shows the specimen in the coldest position (560째C). Some deposits are seen.
Other Alloys Loop 18A. After a problem resulting from a heater short to the loop tubing, loop 18 was drained and the hot leg replaced. New salt was added, and the loop was designated 18A. The operating conditions for loop 18A are listed in Table 1. We placed several alloys with improved resistance to cracking by tellurium in fuel salt in the loop (NCL-18A) to determine their relative compatibility. Tables 9 and 10 show the alloys tested, their compositions, and the total weight change. Figure 35 shows the time dependence of the weight changes. The weight change results show a correlation between corrosion resistance and alloy constituents that form stable fluorides. There is, of course, a rather good correlation between weight changes and chromium or iron content. The nickel-base alloys are far more resistant to corrosion than the iron-base alloy. It is not possible to obtain absolute corrosion information from a test with so many materials present, but the detrimental effects of increasing chromium and iron are obvious. If the loop had been constructed entirely of one of the test alloys, the corrosion rate of the alloy might not have been as large as we noted in our experiment. The less-corrosion-resistant material always suffers in comparison with the corrosion-resistant material when they are in the same system. The microstructures of the alloys are shown in Fig. 36. No attack is seen on the Hastelloy N, and there is little attack on the Inconel 600. You will note a layer of deposit on the Monel with voids underneath. Table 9. Compositions of test alloys Ni Monel HastelloyN Inconel600 Inconel606 Inconel601 Inconel690 Incoloy811E
65 -70 -75 -70 -60 -50 -30
C k F e M o C u A l N b M n
35 7 15 20 23 30 21
7 2 14 15 47
Table 10. Weight changes of alloys exposed to LiF-BeFz-ThF4-UF4 (68-2G11.7-0.3 mole %) at 690째C for 2776 hr
Monel Hastelloy N Inconel 600 Inconel 606 Inconel 601 Inconel 690 Incoloy 811E
0 7 15 20 23 30 21
5 7 2 14 15 47
Total active alloying constituentsa
Weight change (mg/cm2)
(%I 2 14 25 27 38 45 70
M.78 -0.15 -0.49 -6.6 -16.0 -555 -116.7
aConstituents that tend to form, rather stable fluorides. All corrosion s p e c i m p were annealed 1 hr at 1121 C except Monel, which was annealed 1hr at 800 C.
Since the composition of the Monel alloy is most unlike that of any of the other alloys, it is reasonable to assume that after some initial attack, some material deposited on the Monel by an activity gradient transfer mechanism, thus causing the weight gain that we measured. Thus the Monel was not quite as corrosion resistant as our weight changes showed. The cross-section view of the Inconel 606 is unusual since at one end of the specimen we see heavy attack while at the other end almost no attack. This corrosion specimen was not placed any differently in the loop, so its behavior is not completely understood. We would suspect that there might be a homogeneity problem in the specimen. The attack of the Inconel 601,Inconel 690, and the Incoloy 811E was more straightforward and resulted in large areas of void formation: 5 m i l s for Inconel 601,15mils for Inconel 690,and 18 mils for Incoloy 81 1E. ORNL-DWG 73-9847R
OPERATION TIME (hr) I
AT THIS TlMErImpy
Fig. 35. Weight changes of various alloys exposed to LiF-BeFz-ThF4-UF4(68-20.11.7-0.3 mole %) at 69OoCin loop 18.
Fig. 36. Microstructures of various alloys exposed to LiF-BeF2-ThF4-UF4(68-20-11.74.3 mole %) at 69OoC for 2776 hr. (a) Hastelloy N, 500X; (b) Monel, 500X; (c) Inconel 600, SOOX;(d) Inconel 606,1OOX;(e) Inconel 601,lOOX; u> Inconel 690,lOOX; (g) Incoloy 811E, 1OOX. Reduced 24.5%.
1. Temperature gradient mass transfer, as noted by weight losses in the hot leg and weight gains in the cold leg, was evidenced in all systems tested. 2. The weight changes of corrosion specimens increased with increasing temperature and time. 3. Some difficulty was encountered in melting LiF-BeFp-ThF4 salt which was frozen in a loop. The difficulty stemmed from its high melting point and the high melting point of certain phases in the salt. 4. Repairs and welds were made on tubing which had been exposed to molten fluoride salts. 5. All the salts tested were compatible with Hastelloy N. 6. Bismuth in contact with a fuel salt had no effect on mass transfer in a Hastelloy N loop. 7. We established that electrochemical methods to determine the oxidation potential of molten fluoride salts/could be used on a thermal convection loop. The values obtained by the electrochemical methods correlated well with specimen weight change data. 8. We showed that tellurium (as plated on Hastelloy N specimens) does mass transfer in a molten fluoride salt system and that an equilibrium between tellurium in the salt and tellurium on the alloy can be established. 9. A type 304L stainless steel exposed to a fuel salt for 9.5 years in a type 304L stainless steel loop showed a maximum uniform corrosion rate of 0.86 mil/year. Voids extended into the matrix for 10 mils. Chromium depletion was found. 10. The corrosion resistance of a maraging steel (12% Ni-5% Cr-3% Mo-bal Fe) at 662째C was better than type 304L stainless but worse than Hastelloy N under equivalent conditions. The uniform corrosion rate was 0.55 mil/year. Voids were seen in the microstructure of the specimens after 5700 hr, and microprobe analysis disclosed a definite depletion of chromium and iron. 11. Type 316 stainless steel exposed to a fuel salt in a type 3 16 stainless steel loop showed a maximum uniform corrosion rate of 1 mil/year for 4298 hr. Mass transfer did occur in the system. 12. For selected nickel- and iron-base alloys a direct correlation was found between corrosion resistance in a molten fluoride salt and chromium and iron content of an alloy. The more chromium and iron in the alloy, the less corrosion resistance.
O R N L-TM-4286 1 (c
INTERNAL DISTRIBUTION (79 copies)
(5) J. W. Koger E. J. Lawrence A. L. Lotts T. S. Lundy R. N. Lyon H. G. MacPherson R. E. MacPherson W. R. Martin R. W. McClung H. E. McCoy C. J. McHargue H.A. McLain B. McNabb L. E. McNeese A. S. Meyer R. B. Parker P. Patriarca A. M. Perry M. W. Rosenthal H. C. Savage J. L. Scott J. H. Shaffer G.M. Slaughter G.P. Smith R. A. Strehlow R. E. Thoma D. B. Trauger A. M. Weinberg
(3) Central Research Library ORNL - Y-12 Technical Library Document Reference Section (IO) Laboratory Records Department Laboratory Records, ORNL RC ORNL Patent Office G. M. Adamson, Jr. C. F. Baes C. E. Bamberger S. E. Beall E. G. Bohlmann R. B. Briggs S. Cantor E. L. Compere W. H. Cook F. L. Culler J. E. Cunningham J. M. Dale J. H. DeVan J. R. DiStefano J. R. Engel D. E. Ferguson J. H. Frye, Jr. L. 0. Gilpatrick W. R. Grimes A. G. Grindell W. 0. Harms P. N. Haubenreich (3) M. R. Hill W. R. Huntley H. Inouye P. R. Kasten
J. C. White L.V. Wilson
EXTERNAL DISTRIBUTION (24 copies)
BABCOCK & WILCOX COMPANY, P. 0. Box 1260, Lynchburg, VA 24505 B. Mong .*
BLACK AND VEATCH, P. 0. Box 8405, Kansas City, MO 641 14 C. B. Deering BRYON JACKSON PUMP, P. 0. Box 2017, Los Angeles, CA 90054 G. C. Clasby CABOT CORPORATION, STELLITE DIVISION, 1020 Park Ave., Kokomo, IN 46901 T. K. Roche
CONTINENTAL OIL COMPANY, Ponca City, OK 74601 J. A. Acciarri
EBASCO SERVICES, INC., 2 Rector Street, New York, NY 10006 D. R. deBoisblanc T. A. Flynn
THE INTERNATIONAL NICKEL COMPANY, Huntington, WV 25720 J. M. Martin UNION CARBIDE CORFORATION, CARBON PRODUCTS DIVISION, 12900 Snow Road, Parma, OH 44130 R. M. Bushong USAEC, DIVISION OF REACTOR DEVELOPMENT AND TECHNOLOGY, Washington, DC 20545 David Elias J. E. Fox Norton Haberman C. E. Johnson T. C. Reuther S. Rosen Milton Shaw J.M. Simmons . USAEC, DIVISION OF REGULATIONS, Washington, DC 20545 A. Giambusm USAEC, RDT SITE REPRESENTATIVES, Oak Ridge National Laboratory, P. 0. Box X, Oak Ridge, D. F. Cope Kermit Laughon C. L. Matthews USAEC, OAK RIDGE OPERATIONS, P. 0. Box E, Oak Ridge, TN 37830 Research and Technical Support Division USAEC, TECHNICAL INFORMATION CENTER, P. 0. Box 62, Oak Ridge, TN 37830 (2)
*US. G O V E R N M E N T P R I N T I N G OFFICE: 1973-747-302170